Download presentation

Presentation is loading. Please wait.

Published byPercival Tucker Modified about 1 year ago

1
Characterization and modeling the thermo- mechanical cure-dependent properties of epoxy molding compound Reporter: Shi Lei Date:2012.6

2
2 Outlines Introduction Materials and sample preparation DSC experiment PVT measurement Dynamic Mechanical Analyzer (DMA) Conclusions

3
Introduction Epoxy molding compounds (EMCs) for semiconductor are used for protecting semiconductor chips from external environment, specifically from external physical forces such as impact and pressure, and external chemical forces such as moisture, heat, and ultraviolet ray, maintaining the electric insulating property, and providing the semiconductor package with a form allowing easier mounting on a print circuit board. Failure in microelectronics packaging mostly happens through polymer cracking, interface delamination and thermal fatigue, caused mainly by thermo-mechanical loadings. And stresses generate during the curing and cooling of the molding compound. Therefore, investigating the thermo-mechanical cure-dependent properties of EMC has become more and more important.

4
Materials and sample preparation 4 The matrix material: Epoxy Novolac (EPN1180, Huntsman Advanced Materials, equivalent weight 175–182 g/eq) The hardener: Bisphenol-A (equivalent weight 114 g/eq) The filler: fused silica spheres (FB-940, exDenka, median diameter 15 mm, density2.20 g/cm3) The catalyst : Triphenylphosphine (TPP, 0.5g/100gepoxy). The epoxy Novolac and Bisphenol-A were mixed in a stoichiometric ratio. Two materials were used in these experiments: The unfilled (with 0% filler) and the filled one with 64.5wt% (50vol%) filler.

5
DSC experiment 5 Differential Scanning Calorimetry (DSC) was used to obtain curing process parameters, such as the degree and rate of chemical conversion and the glass transition temperature. The degree of conversion was modeled with the auto- catalytic Kamal–Sourour equation : The unknown parameters m and n as well as k0 and Ea were determined by analyzing temperature scans on non-reacted materials from 0 to 200 ℃ at heating rates of 5,10 and 15 ℃ /min.

6
6 As it shows Htot in different heating rates is almost constant for filled and unfilled materials separately. However the peak of the released heat increases within creasing heating rates. As an additional check we estimated the reaction heat for the filled sample, based on that for the unfilled samples and the known filler content (64.5 wt%), assuming that the filler is inert and does not contribute to the released heat. The last row of Table 1 shows that this assumption is indeed justified.

7
7 The predicted results of Kamal–Sourour equation show that the reaction is much slower in filled materials. This effect can be interpreted as a partial deactivation of the catalyst by the silica filler. This shows that there is a good agreement between the conversion predictions and the experimental values from the isothermal cure tests.

8
8 The glass transition temperature curves were fitted to the empirical DiBenedetto model :

9
PVT measurement 9 A GNOMIX high pressure dilatometer (PVT Apparatus) was used to determine the amount of volumetric decrease due to the curing. The graph is divided into three major parts: increase in volume during heating, subsequent isothermal cure shrinkage and cooling down to room temperature. The total cure shrinkage can be calculated from the difference of the values at the end and starting time of the cure. Due to the filler, the cure shrinkage of the filled material is less than the unfilled one (2.1 vs. 3.4 vol%).

10
10 Fig. 6 shows that the cure shrinkage’s curves are approximately linear. For practical purposes we neglect these deviations and approximate the cure shrinkage as being linear with conversion, Eq. (3). The result of the model is also shown in Fig. 6.

11
11 The high pressure dilatometer was also used to determine the coefficient of thermal expansion (CTE) of the fully cured EMC. The volume change of the fully cured filled molding compounds is shown in Fig. 7. The results clearly show a linear volume increase in the glassy region and a second linear region above Tg.

12
12 As a model we use the well known Tait equation: The volumetric CTE then follows by differentiating with respect to temperature, resulting in:

13
13 Since it is more customary to work with the linear coefficients of thermal expansion we defined those as 1/3 of the volumetric ones. This shows that the glassy and rubbery CTE of the filled samples is almost 45% of that of the unfilled sample, which matches quite well with expectation.

14
14 The compressibility can be determined in a similar way as for the CTE but now by differentiating with respect to volume: The bulk modulus is obtained here as the inverse of the bulk compressibility: Due to filler, the glassy and rubbery bulk moduli of the filled sample become, respectively, 2.4 and 2 times higher than unfilled one.

15
Dynamic Mechanical Analyzer (DMA) 15 A Dynamic Mechanical Analyzer, TA Q800, was used to measure the viscoelastic elongation behavior of filled and unfilled fully cured samples as a function of the excitation frequency and temperature. Fig. 10 clearly shows that for each material, Eg (Elongation glassy modulus) and Er (Elongation rubbery modulus) are independent of the frequency. However in the glass transition regime clear frequency dependent effects can be seen. If we take the peak position of 1Hz tan d curves as the DMA glass transition temperature, we obtain values of 128 ℃ and 121 ℃ for the unfilled and filled material, respectively.

16
16 The storage modulus can be interpolated and plotted as a function of frequency and temperature, Fig. 11. Time–temperature super- position appears to be valid for the fully cured filled and unfilled materials.

17
17 Below the switching temperature, Tc, the shift factor follows the Arrhenius behavior (activation energy driven), Eq.(9), whereas above this temperature it follows the WLF behavior (free volume mechanism), Eq.(10).

18
Conclusions 18 In this paper an extensive study on the thermo-mechanical cure-dependent properties of a series of epoxy resins with and without filler was carried out. The effect of the filler was also investigated on these thermo-mechanical properties and the result shows that the filler decreases the cure shrinkage and thermal contraction of epoxy resins but increases the modulus below and above the glass transition temperature. Thanks for your attention!

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google